Section 04720 Cast Stone
1. PART 1 - GENERAL
1.1. SECTION INCLUDES - Architectural Cast Stone.
A. Description, design requirements, fabrication, and installation.
1. Manufacturer shall furnish Cast Stone covered by this specification.
2. Installing contractor shall unload, store, furnish all anchors, set, patch, clean and seal
(optional) the Cast Stone as required.
1.2. RELATED SECTIONS
A. Section – 01 33 00 – Submittal Procedures.
B. Section – 04 05 13 – Masonry Mortaring.
C. Section – 04 05 16 – Masonry Grouting.
D. Section – 04 05 19 – Masonry Anchorage and Reinforcing.
E. Section – 07 90 00 – Joint Protection.
A. ACI 318 – Building Code Requirements for Reinforced Concrete.
B. ASTM A 185 - Standard Specification for Steel Welded Wire Reinforcement, Plain, for
C. ASTM A 615/A 615M - Standard Specification for Deformed and Plain Billet-Steel Bars for
D. ASTM C 33 – Standard Specification for Concrete Aggregates.
E. ASTM C 150 - Standard Specification for Portland Cement.
F. ASTM C 173 - Standard Test Method for Air Content of Freshly Mixed Concrete by the
G. ASTM C 231 - Standard Test Method for Air Content of Freshly Mixed Concrete by the
H. ASTM C 260 - Standard Specification for Air-Entrained Admixtures for Concrete.
I. ASTM C 270 - Standard Specification for Mortar for Unit Masonry.
J. ASTM C 426 – Standard Test Method for Linear Shrinkage of Concrete Masonry Units
K. ASTM C 494/C 494M - Standard Specification for Chemical Admixtures for Concrete.
L. ASTM C 618 – Specification for Coal Fly Ash and Raw or Calcined Natural Pozzolan for Use
as a Mineral Admixture in Concrete.
M. ASTM C 666 – Standard Test Method for Resistance of Concrete to Rapid Freezing and
N. ASTM C 979 - Standard Specification for Coloring Pigments for Integrally Pigmented
O. ASTM C 989 – Standard Specification for Ground Granulated Blast-Furnace Slag for Use in
P. ASTM C 1194 - Standard Test Method for Compressive Strength of Architectural Cast
Q. ASTM C 1195 - Standard Test Method for Absorption of Architectural Cast Stone.
R. ASTM C 1364 - Standard Specification for Architectural Cast Stone.
S. ASTM D 2244 – Standard Test Method for Calculation of Color Differences from
Instrumentally Measured Color Coordinates.
T. Cast Stone InstituteSM Technical Manual (Current Edition)
A. Cast Stone - a refined architectural concrete building unit manufactured to simulate
natural cut stone, used in unit masonry applications.
1. Dry Cast Concrete Products – manufactured from zero slump concrete.
a. Vibrant Dry Tamp (VDT) casting method: Vibratory ramming of earth moist,
zero- slump concrete against a rigid mold until it is densely compacted.
1.5. SUBMITTAL PROCEDURES
A. Comply with Section 01 33 00 – Submittal Procedures.
B. Samples: Submit pieces of the Cast Stone 6” x 6” x 1” exemplifying color, and texture to
be used in project.
C. Test results: Submit manufacturers test results of Cast Stone previously made by the
D. Shop Drawings: Submit manufacturers shop drawings including profiles, cross-sections,
reinforcement, exposed faces, arrangement of joints (optional for standard or semi-
custom installations), anchoring methods, anchors (if required), annotation of stone types
and their location.
1.6. QUALITY ASSURANCE
A. Manufacturer Qualifications:
1. Manufacturer should be a current member of the Cast Stone Institute, with a
minimum of 5 years continuous successful experience in fabricating architectural cast
stone with demonstrated abilities, facilities and manufacturing capacity required to
furnish cast stone requirements of this project without delay of work in progress.
B. Standards: Comply with the requirements of the Cast Stone InstituteSM Technical Manual
and the project specifications. Where a conflict may occur, the contract documents shall
C. Mock-up (Optional) Provide full size unit(s) for use in construction of sample wall. The
approved mock-up shall become the standard for appearance and workmanship for the
2. PART 2 - PRODUCTS
2.1. ARCHITECTURAL CAST STONE- Acceptable Manufacturer:
A. Cast Stone Systems, Inc. Warrenton, North Carolina 888-501-5204,
A. Comply with ASTM C 1364
B. Physical properties: Provide the following:
1. Compressive Strength - ASTM C 1194: 6,500 psi (45 Mpa) minimum for products at 28
2. Absorption - ASTM C 1195: 6% maximum by the cold water method, or 10%
maximum by the boiling method for products at 28 days.
3. Air Content – ASTM C173 or C 231, for wet cast product shall be 4-8% for units
exposed to freeze-thaw environments. Air entrainment is not required for VDT
4. Freeze-thaw – ASTM C 1364: The CPWL shall be less than 5% after 300 cycles of
freezing and thawing.
5. Linear Shrinkage – ASTM C 426: Shrinkage shall not exceed 0.065%.
C. Job site testing – One (1) sample from production units may be selected at random from
the field for each 500 cubic feet (14 m 3) delivered to the job site.
1. Three (3) field cut cube specimens from each of these samples shall have an average
minimum compressive strength of not less than 85% with no single specimen testing
less than 75% of design strength as allowed by ACI 318.
2. Three (3) field cut cube specimens from each of these samples shall have an average
maximum cold-water absorption of 6%.
3. Field specimens shall be tested in accordance with ASTM C 1194 and C 1195.
2.2. RAW MATERIALS
A. Portland cement – Type I or Type III, white and/or grey, ASTM C 150.
B. Coarse aggregates - Granite, quartz or limestone, ASTM C 33, except for gradation, and
are optional for the VDT casting method.
C. Fine aggregates - Manufactured or natural sands, ASTM C 33, except for gradation.
D. Colors - Inorganic iron oxide pigments, ASTM C 979 except that carbon black pigments
shall not be used.
E. Admixtures- Comply with the following:
1. ASTM C 260 for air-entraining admixtures.
2. ASTM C 494/C 495M Types A - G for water reducing, retarding, accelerating and high
3. Other admixtures: integral water repellents and other chemicals, for which no ASTM
Standard exists, shall be previously established as suitable for use in concrete by
proven field performance or through laboratory testing.
4. ASTM C 618 mineral admixtures of dark and variable colors shall not be used in
surfaces intended to be exposed to view.
5. ASTM C 989 granulated blast furnace slag may be used to improve physical properties.
Tests are required to verify these features.
F. Water – Potable
G. Reinforcing bars:
1. ASTM A 615/A 615M. Grade 40 or 60 steel galvanized or epoxy coated when cover is
less than 1.5 in. (37 mm).
2. Welded Wire Fabric: ASTM A 185 where applicable for wet cast units.
H. All anchors, dowels and other anchoring devices and shims shall be standard building
stone anchors commercially available in a non-corrosive material such as zinc plated,
galvanized steel, brass, or stainless steel Type 302 or 304.
2.3. COLOR AND FINISH
A. Generally match sample on file at Architects office.
B. All surfaces intended to be exposed to view shall have a fine-grained texture similar to
natural stone, with no air voids in excess of 1/32 in. (0.8 mm) and the density of such
voids shall be less than 3 occurrences per any 1 in.2 (25 mm2) and not obvious under
direct daylight illumination at a 5 ft (1.5m) distance.
C. Units shall exhibit a texture approximately equal to the approved sample when viewed
under direct daylight illumination at a 10 ft (3 m) distance.
1. ASTM D 2244 permissible variation in color between units of comparable age subjected
to similar weathering exposure.
a. Total color difference – not greater than 6 units.
b. Total hue difference – not greater than 2 units.
D. Minor chipping resulting from shipment and delivery shall not be grounds for rejection.
Minor chips shall not be obvious under direct daylight illumination from a 20-ft (6 m)
E. The occurrence of crazing or efflorescence shall not constitute a cause for rejection.
F. Remove cement film, if required, from exposed surfaces prior to packaging for shipment.
A. Reinforce the units as required by the drawings and for safe handling and structural
B. Minimum reinforcing shall be 0.25 percent of the cross section area.
C. Reinforcement shall be noncorrosive where faces exposed to weather are covered with
less than 1.5 in. (38 mm) of concrete material. All reinforcement shall have minimum
coverage of twice the diameter of the bars.
D. Panels, soffits and similar stones greater than 24 in. (600 mm) in one direction shall be
reinforced in that direction. Units less than 24 in. (600 mm) in both their length and
width dimension shall be non-reinforced unless otherwise specified.
E. Welded wire fabric reinforcing shall not be used in dry cast products.
A. Cure units in a warm curing chamber at 95 percent relative humidity for approximately
12 hours, or cure in a 95 percent moist environment at a minimum 70ºF (21.1ºC) for 16
hours after casting. Additional yard curing at 95 percent relative humidity shall be 350
degree-days (i.e. 7 days @ 50°F (10°C) or 5 days @ 70°F (21°C)) prior to shipping. Form
cured units shall be protected from moisture evaporation with curing blankets or curing
compounds after casting.
2.6. MANUFACTURING TOLERANCES
A. Cross section dimensions shall not deviate by more than ±1/8 in. (3 mm) from approved
B. Length of units shall not deviate by more than length/ 360 or ±1/8 in. (3 mm), whichever
is greater, not to exceed ±1/4 in. (6 mm).
1. Maximum length of any unit shall not exceed 15 times the average thickness of such
unit unless otherwise agreed by the manufacturer.
C. Warp, bow or twist of units shall not exceed length/ 360 or ±1/8 in. (3 mm), whichever is
D. Location of dowel holes, anchor slots, flashing grooves, false joints and similar features –
On formed sides of unit, 1/8 in. (3 mm), on unformed sides of unit, 3/8 in. (9 mm)
2.7. PRODUCTION QUALITY CONTROL
1. Test compressive strength and absorption from specimens selected at random from
2. Samples shall be taken and tested from every 500 (14 m3) cubic feet of product
3. Perform tests in accordance ASTM C 1194 and C 1195.
4. New and existing mix designs shall be tested for strength and absorption compliance
prior to producing units.
2.8. DELIVERY, STORAGE AND HANDLING
A. Mark production units with the identification marks as shown on the shop drawings.
B. Package units and protect them from staining or damage during shipping and storage.
C. Provide an itemized list of product to support the bill of lading.
3. PART 3 EXECUTION
A. Installing contractor shall check Cast Stone materials for fit and finish prior to installation.
Do not set unacceptable units.
3.2. SETTING TOLERANCES
A. Comply with Cast Stone InstituteSM Technical Manual.
B. Set stones 1/8 in. (3 mm) or less, within the plane of adjacent units.
C. Joints, plus - 1/16 in. (1.5 mm), minus - 1/8 in. (3 mm).
A. Joint size:
1. At stone/brick joints 3/8 in. (9.5 cm).
2. At stone/stone joints in vertical position 1/4 in. (6 mm) (3/8 in. (9.5 mm) optional).
3. Stone/stone joints exposed on top 3/8 in. (9.5 mm).
B. Joint materials:
1. Mortar, Type N, ASTM C 270.
2. Use a full bed of mortar at all bed joints.
3. Flush vertical joints full with mortar.
4. Leave all joints with exposed tops or under relieving angles open for sealant.
5. Leave head joints in copings and projecting components open for sealant.
C. Location of joints:
1. As shown on shop drawings.
2. At control and expansion joints unless otherwise shown.
A. Drench units with clean water prior to setting.
B. Fill dowel holes and anchor slots completely with mortar or non-shrink grout.
C. Set units in full bed of mortar, unless otherwise detailed.
D. Rake mortar joints 3/4 in. (18 mm) in. for pointing.
E. Remove excess mortar from unit faces immediately after setting.
F. Tuck point unit joints to a slight concave profile.
3.5. JOINT PROTECTION
A. Comply with requirements of Section 07 90 00.
B. Prime ends of units, insert properly sized backing rod and install required sealant.
3.6. REPAIR AND CLEANING
A. Repair chips with touchup materials furnished by manufacturer.
B. Saturate units to be cleaned prior to applying an approved masonry cleaner.
C. Consult with manufacturer for appropriate cleaners.
3.7. INSPECTION AND ACCEPTANCE
A. Inspect finished installation according to Bulletin #36.
B. Do not field apply water repellant until repair, cleaning, inspection and acceptance is